Toward a comprehensive understanding of solid-state core ... · PDF fileToward a comprehensive...
Embed Size (px)
Transcript of Toward a comprehensive understanding of solid-state core ... · PDF fileToward a comprehensive...
Toward a comprehensive understanding of solid-state core-level XPS linewidths: Experimentaland theoretical studies on the Si 2p and O 1s linewidths in silicates
G. M. Bancroft,1,* H. W. Nesbitt,2 R. Ho,2 D. M. Shaw,3 J. S. Tse,3 and M. C. Biesinger41Department of Chemistry, University of Western Ontario, London, Ontario, Canada N6A 5B7
2Department of Earth Sciences, University of Western Ontario, London, Ontario, Canada N6A 5B73Department of Physics, University of Saskatchewan, Saskatoon, Saskatchewan, Canada S7N 5E2
4Surface Science Western, University of Western Ontario, London, Ontario, Canada N6A 5B7Received 28 April 2009; published 4 August 2009
High resolution X-ray Photoelectron Spectroscopy XPS core-level Si 2p and O 1s spectra of the noncon-ductors -SiO2 quartz at 120 and 300 K and vitreous SiO2 at 300 K were obtained with a Kratos Axis UltraXPS instrument instrumental resolution of 0.4 eV which incorporates a unique charge compensation sys-tem that minimizes differential charge broadening on nonconductors. The Si 2p and O 1s linewidths at 300 K1.1 and 1.2 eV, respectively are similar for all silicates and similar to previous thin film SiO2 spectraobtained previously, showing that differential charging does not contribute significantly to our spectra. At 120K, there is a small decrease 0.04 eV in the Si 2p linewidth of -SiO2, but no measurable decrease in O 1slinewidth. The O 1s lines are generally and distinctly asymmetric. We consider all possible sources of linebroadening and show that final state vibrational broadening FSVB and phonon broadening are the majorcauses of the broad and asymmetric lines. Previous high resolution gas phase XPS studies have identified largeFSVB contributions to the Si 2p spectra of SiCl4, SiF4, and SiOCH34 molecules, and this vibrational structureleads total Si 2p3/2 linewidths of up to 0.5 eV, even with individual peak linewidths of 0.1 eV. The Siatom of SiOCH34 is an excellent analog for Si in crystalline SiO2 because the Si-O bond lengths andsymmetric stretch frequencies are similar in both compounds. Similar vibrational contributions to the Si 2p andO 1s spectra of solid silicates are anticipated if the Si 2p and O 1s core-hole states produce similar changes tothe Si-O bond length in both phases. To investigate the possibility, Car-Parrinello molecular dynamics calcu-lations were performed and show that changes to Si-O bond lengths between ion and ground states r forboth Si 2p and O 1s hole states are similar for both crystalline SiO2 and gaseous SiOCH34. r are 0.04 for Si 2p and +0.05 for O 1s in both compounds. Indeed, the vibrational envelope from the Si 2pspectrum of SiOCH34, broadened to our instrumental linewidth of 0.4 eV, accounts for the majority0.8 eV of the Si 2p3/2 linewidth for crystalline SiO2 1.1 eV with phonon broadening accounting forthe remainder. The results provide excellent support for the tenet that final state vibrational splitting, as seen inthe gas phase molecules, similarly affects the solid-state spectra. The calculations also indicate that the O 1slinewidths should be larger than the Si 2p linewidths, as observed in our spectra. FSVB should also lead tosmall peak asymmetries, as seen in the O 1s spectra. The contribution of phonon broadening to the linewidthis also evaluated and shown to be comparable to the FSVB contribution at 120 and 300 K but considerablysmaller at very low temperatures.
DOI: 10.1103/PhysRevB.80.075405 PACS numbers: 79.60.Bm, 71.15.Mb
O 1s X-ray Photoelectron Spectroscopy XPS spectraand core-level spectra of many other elements in oxides arewidely used to obtain chemical state information of oxygenand metal species in and on solids and surfaces before andafter chemical reactions. With the advent of high resolutionsynchrotron x-ray sources, high resolution electron analyz-ers, and effective charge neutralization systems e.g., KratosAxis Ultra instrument which dramatically decrease chargebroadening for rough nonconductor surfaces, experimentalcore-level spectra are now highly reproducible for nearly alltypes of solid surfaces. Core-level XPS spectra and particu-larly O 1s spectra consequently have been used ever morewidely to characterize bulk and thin film simple oxides e.g.,see very recent references to pristine, thin films, modifiedthin films, or reacted surfaces such as TiO2,
17 SiO2 andsilicates,813 RuO2,
14,15 MgO,1618 CaO,19 ZnO,20 Fe3O4,21
Cu2O,22 and other transition metal oxides;2325 also see a
recent review of ambient pressure XPS on oxides26.
Recent XPS studies on nonconductor glasses,2730 com-plex superconductor oxides,3133 ceramics,34,35 and surfacereactions of many oxygen-containing molecules on a widevariety of substances3639 have also reported narrower O 1sand other core-level linewidths than previously collected.Because the majority of these substrates are nonconductors,many recent studies have been conducted using the Kratosinstrument with its novel magnetic confinement charge com-pensation system. The instrument has yielded reproducibleO 1s and other core-level spectral line shapes and linewidthson both atomically smooth and rough nonconductor surfaces:the O 1s linewidths, for example, are often muchnarrower811,2729 than previously obtained with other instru-ments for bulk nonconductors. Moreover, nonconductor line-widths have been shown to be just as narrow as obtained forsemiconductors8 or metals.40 For example,40 VO2 exhibits aninsulator-metal transition above 300 K and the O 1s line-width at 270 K of the insulator phase of VO2 measured fromFig. 3 of Ref. 40 as 1.0 eV is as narrow as or slightlynarrower than the linewidth of the metallic phase at 320 K
PHYSICAL REVIEW B 80, 075405 2009
1098-0121/2009/807/07540513 2009 The American Physical Society075405-1
measured as at least 1.1 eV. O 1s linewidths for the metal-lic phase are difficult for us to simply measure off a pub-lished figure because of the Doniach-Sunjic asymmetry,which was not quantified in Ref. 40.
Although surface charging has been largely overcomewith technical advances, core-level linewidths of oxides re-main surprisingly large. In most of the above studies, theO 1s and other core-level spectra were fitted with symmetricGaussian/Lorentzian or Voigt line shapes and fits yieldedO 1s linewidths commonly greater than 1.0 eV e.g., about1.2 eV for silicates811,2729 and about 1.4 eV for MgO Refs.1618. The O 1s linewidths on the semiconductor TiO2and other transition metal oxides and superconductors arenarrower, but still usually 1.0 eV, except for Cu2O,
RuO2,14,15 and the superconductors Sr2CuO2Cl2 and
Ca2CuO2Cl2.33 The O 1s linewidths on the bulk semiconduc-
tor Cu2O Ref. 22 at room temperature appear to be thenarrowest O 1s linewidth yet published at 0.7 eV; while formetallic RuO2 films
14,15 the O 1s linewidths at 100 K were0.75 eV both results obtained with high resolution syn-chrotron radiation sources with a total experimental reso-lution of less than 0.2 eV. It is also apparent from Si 2p3/2spectra of silicates, Ti 2p3/2 spectra for TiO2, and Ru 3d5/2spectra of RuO2 that the metal linewidths are usually nar-rower than the O 1s linewidths for a given compound. In-deed, the Ru 3d3/2 linewidth of the conducting RuO2 films onRu metal is 0.5 eV, whereas the O 1s linewidth is0.75 eV.
In addition to broad lines, some O 1s spectra e.g., MgO,CaO, and silicates display a small but distinct asymmetrymaking it necessary to fit an additional peak 1020 % of theintensity of the main peak usually on the high binding en-ergy side of the peak.13,28 The high energy peak has some-times been assigned to an additional chemicalspecies.13,28,35,39
Questions arise from the above results: 1 why are theseO 1s linewidths so broad and variable 0.7 to 1.3 eV rela-tive to observed individual linewidths of 50150 meV forSi 2p, C 1s, P 2p, and B 1s spectra of polyatomic moleculesin the gas phase;4145 2 why are they much broader thantotal linewidths observed for semiconductor solids such asSi,4648 PbS Ref. 49 0.3 eV, FeAsS and FeS2 Ref. 500.5 eV, and for other nonconductors such as As2S3 Ref.8 0.5 eV; 3 should the O 1s line shapes be symmetricwhen there is only one structural O species in an oxide; and4 why are the metal linewidths generally narrower than theO 1s linewidths for a given oxide?
Traditionally, large solid-state linewidths have been attrib-uted to phonon broadening PB. In 1974, Citrin et al.51 pub-lished temperature dependent monochromatic XPS spectra ofthe potassium and halide core levels on thin film potassiumhalides. The measured linewidths of about 1 eV were cor-rected for the instrumental effects photon and electron line-widths. The temperature dependence of the nonconductorlinewidths better seen in the core-level metal spectra51 wasshown to be consistent5153 with phonon broadening fromexcitation of a large number of phonons produced in re-sponse to hole production. Phonon broadening should lead tosymmetric Gaussian5153 line shapes, and there was no evi-dence for asymmetry in the experimental spectra of the alkali
halides. The phonon contribution explained the temperaturedependence of the linewidths, but the corrected experimentallinewidths were, at all temperatures, larger than calculated,51
with no explanation provided. Furthermore, separate calcula-tions yielded large differences 0.2 eV in the calculatedlinewidths.5153 Finally, the linewidths extrapolated to 0 Khere referred to as PH0 have large uncertainties becauseextrapolations of experimental data extended over an300 C range.
The extrapolations, nevertheless, indicate PH0 valuesmuch greater than inherent linewidths expected from finalstate lifetime contributions.
Another possible major contribution